 
data_p4bymnc_sq
 
_audit_creation_method            SHELXL-2014
_chemical_name_systematic
;
 ?
;
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          
'O118 U28'
_chemical_formula_sum
 'O118 U28' 
_chemical_formula_weight          8552.84

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'U'  'U'  -9.6767   9.6646
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       tetragonal
_space_group_IT_number            128
_space_group_name_H-M_alt         'P 4/m n c'
_space_group_name_Hall            '-P 4 2n'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 '-y, x, z'
 '-x, -y, z'
 'y, -x, z'
 'x+1/2, -y+1/2, -z+1/2'
 '-x+1/2, y+1/2, -z+1/2'
 'y+1/2, x+1/2, -z+1/2'
 '-y+1/2, -x+1/2, -z+1/2'
 '-x, -y, -z'
 'y, -x, -z'
 'x, y, -z'
 '-y, x, -z'
 '-x-1/2, y-1/2, z-1/2'
 'x-1/2, -y-1/2, z-1/2'
 '-y-1/2, -x-1/2, z-1/2'
 'y-1/2, x-1/2, z-1/2'
 
_cell_length_a                    20.234(3)
_cell_length_b                    20.234(3)
_cell_length_c                    26.874(5)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma                 90
_cell_volume                      11002(4)
_cell_formula_units_Z             2
_cell_measurement_temperature     100(2)
_cell_measurement_reflns_used     9980 
_cell_measurement_theta_min       2.5
_cell_measurement_theta_max       22.5 
 
_exptl_crystal_description        'plates'
_exptl_crystal_colour             'plates'
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_method     ?              
_exptl_crystal_density_diffrn     2.582          
_exptl_crystal_F_000              7040
_exptl_transmission_factor_min    ?                                             
_exptl_transmission_factor_max    ?                                             
_exptl_crystal_size_max           0.015
_exptl_crystal_size_mid           0.010
_exptl_crystal_size_min           0.010
_exptl_absorpt_coefficient_mu     20.582
_shelx_estimated_absorpt_T_min    0.748
_shelx_estimated_absorpt_T_max    0.821
_exptl_absorpt_correction_type    'Multi-scans'  
_exptl_absorpt_correction_T_min   ? 
_exptl_absorpt_correction_T_max   ? 
_exptl_absorpt_process_details    ? 
 
_exptl_special_details
;
 ?
;
 
_diffrn_ambient_temperature       100(2)
_diffrn_radiation_type           Synchrotron
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Synchrotron BM'
_diffrn_radiation_monochromator  Si<111>
_diffrn_measurement_device_type  '3-BM1 Australian Synchrotron'
_diffrn_measurement_method       'Phi Scan'
_diffrn_detector_type            'ADSC Quantum 210r' 
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_decay_%        0 
_diffrn_reflns_number             132508
_diffrn_reflns_av_unetI/netI      0.0141
_diffrn_reflns_av_R_equivalents   0.0539
_diffrn_reflns_limit_h_min        -23
_diffrn_reflns_limit_h_max        23
_diffrn_reflns_limit_k_min        -24
_diffrn_reflns_limit_k_max        24
_diffrn_reflns_limit_l_min        -31
_diffrn_reflns_limit_l_max        31
_diffrn_reflns_theta_min          1.423
_diffrn_reflns_theta_max          24.998
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.999
_diffrn_measured_fraction_theta_full  0.971
_diffrn_reflns_Laue_measured_fraction_max    0.999
_diffrn_reflns_Laue_measured_fraction_full   0.971
_diffrn_reflns_point_group_measured_fraction_max   0.999
_diffrn_reflns_point_group_measured_fraction_full  0.971
_reflns_number_total              4962
_reflns_number_gt                 4551
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.

 The U28 'ball' in the crystal lattice has two orientations with
 equal occupancies in the crystal lattice, which are rotated by 
 from one anotehr by 90 deg. along the tetragonal (c)axis. This  
 orientational disorder was evident from the uranium peaks that 
 were seen to form a perfect square. Because of the high symmetry
 and the common positions generated in the two orientations, the
 refinement was carried out with both the orientations together,
 that is without separating them in two PARTs. The refinement of 
 oxo and peroxo oxygens with corresponding occupancies was carried 
 out with U=O and U-O bonds restrained to expected average values 
 using DFIX and SADI commands and their atomic displacement 
 parameters with DELU and SIMU commands. The SQUEEZE procedure 
 in PLATON was used in order to remove the contribution from 
 disordered Na ions and waters in the voids generated in packing
 of the U28 balls. 

;
 
_computing_data_collection       'BLU-ICE (McPhillips et al., 2002)'
_computing_cell_refinement       'XDS (Kabsch, 1993)'
_computing_data_reduction        'XDS (Kabsch, 1993)'
_computing_structure_solution    
;
SHELXS97 (Sheldrick, 2008) and OLEX-2 (Dolomanov et al., 2009)
;
_computing_structure_refinement   'SHELXL-2013 (Sheldrick, 2013)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
 
_refine_special_details
;
 ?
;
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.2000P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_number_reflns          4962
_refine_ls_number_parameters      292
_refine_ls_number_restraints      42
_refine_ls_R_factor_all           0.0634
_refine_ls_R_factor_gt            0.0605
_refine_ls_wR_factor_ref          0.2541
_refine_ls_wR_factor_gt           0.2467
_refine_ls_goodness_of_fit_ref    1.246
_refine_ls_restrained_S_all       1.255
_refine_ls_shift/su_max           0.014
_refine_ls_shift/su_mean          0.003
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
U1 U 0.27562(2) 0.59112(3) 0.31906(2) 0.0545(3) Uani 1 1 d D . . . .
U2 U 0.40497(5) 0.45885(6) 0.25938(4) 0.0572(3) Uani 0.5 1 d D U P . .
U3 U 0.22662(4) 0.69498(5) 0.44570(3) 0.0467(3) Uani 0.5 1 d D U P . .
U4 U 0.17040(4) 0.55488(4) 0.44740(3) 0.0456(3) Uani 0.5 1 d D U P . .
U6 U 0.23404(4) 0.38622(4) 0.65198(3) 0.0455(3) Uani 0.5 1 d D U P . .
U5 U 0.18173(3) 0.37154(4) 0.5000 0.0538(3) Uani 1 2 d DS T P . .
O11C O 0.1558(7) 0.3958(9) 0.5846(5) 0.045(4) Uani 0.5 1 d D . P . .
O16C O 0.2000(8) 0.4949(9) 0.6636(7) 0.052(4) Uani 0.5 1 d . . P . .
O15C O 0.2537(11) 0.4740(8) 0.7065(7) 0.070(5) Uani 0.5 1 d D U P . .
O14C O 0.2892(8) 0.2843(8) 0.6701(7) 0.060(4) Uani 0.5 1 d D U P . .
O13C O 0.3103(10) 0.3382(11) 0.7065(5) 0.069(6) Uani 0.5 1 d D U P . .
O12C O 0.1638(12) 0.4437(9) 0.5663(7) 0.073(6) Uani 0.5 1 d D . P . .
O1B O 0.3316(5) 0.5718(7) 0.3672(4) 0.079(3) Uani 1 1 d . . . . .
O1A O 0.2198(5) 0.6143(5) 0.2708(4) 0.061(2) Uani 1 1 d . . . . .
O2C O 0.4875(14) 0.5339(7) 0.2291(6) 0.056(5) Uani 0.5 1 d . . P . .
O2B O 0.4292(11) 0.4726(10) 0.3252(6) 0.069(5) Uani 0.5 1 d D U P . .
O2A O 0.3790(11) 0.4480(15) 0.1950(5) 0.083(7) Uani 0.5 1 d D U P . .
O1C O 0.3483(8) 0.5599(11) 0.2577(6) 0.056(5) Uani 0.5 1 d . . P . .
O4A O 0.0828(7) 0.5630(11) 0.4358(8) 0.068(5) Uani 0.5 1 d D . P . .
O3C O 0.1920(8) 0.5416(9) 0.3609(7) 0.054(4) Uani 0.5 1 d . U P . .
O3B O 0.2979(8) 0.6412(8) 0.4610(6) 0.052(4) Uani 0.5 1 d D U P . .
O3A O 0.1602(9) 0.7516(8) 0.4303(8) 0.067(5) Uani 0.5 1 d D U P . .
O6C O 0.1502(9) 0.6178(9) 0.4804(6) 0.059(4) Uani 0.5 1 d D U P . .
O6B O 0.3020(7) 0.4167(6) 0.6125(5) 0.031(3) Uani 0.5 1 d . . P . .
O6A O 0.1699(11) 0.3596(10) 0.6915(7) 0.063(5) Uani 0.5 1 d . . P . .
O5C O 0.1734(11) 0.6659(7) 0.4749(7) 0.071(6) Uani 0.5 1 d D . P . .
O5B O 0.2637(7) 0.4016(6) 0.5000 0.067(4) Uani 1 2 d S T P . .
O5A O 0.0984(7) 0.3413(10) 0.5000 0.077(4) Uani 1 2 d S T P . .
O4C O 0.1947(5) 0.6187(7) 0.3769(3) 0.032(3) Uani 0.5 1 d D U P . .
O4B O 0.2603(6) 0.5405(10) 0.4587(6) 0.071(6) Uani 0.5 1 d D U P . .
O10C O 0.1870(10) 0.3290(8) 0.5821(5) 0.049(4) Uani 0.5 1 d D . P . .
O9C O 0.2135(8) 0.2969(9) 0.5613(7) 0.055(4) Uani 0.5 1 d D . P . .
O8C O 0.2183(9) 0.2633(6) 0.5000 0.084(5) Uani 1 2 d DS T P . .
O7C O 0.1287(13) 0.4703(9) 0.5000 0.061(6) Uani 0.5 2 d DS TU P . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
U1 O1B 1.764(9) . ?
U1 O1A 1.781(8) . ?
U1 O3C 2.264(18) . ?
U1 O1C 2.298(13) . ?
U1 O4C 2.326(10) . ?
U1 O14C 2.445(17) 10_566 ?
U1 O13C 2.461(14) 10_566 ?
U1 O15C 2.506(19) 11_556 ?
U1 O16C 2.520(18) 11_556 ?
U1 U2 4.0402(14) 4_565 ?
U1 U2 4.0724(14) . ?
U2 O2C 1.589(16) 2_655 ?
U2 O2A 1.823(15) . ?
U2 O2B 1.857(14) . ?
U2 O2C 2.33(3) 3_665 ?
U2 O1C 2.345(19) . ?
U2 O1C 2.347(19) 2_655 ?
U2 O2C 2.40(2) . ?
U2 O2C 2.941(15) 4_565 ?
U2 U2 2.9633(14) 4_565 ?
U2 U2 2.9634(14) 2_655 ?
U2 U1 4.0401(14) 2_655 ?
U3 O5C 1.46(2) . ?
U3 O3A 1.813(14) . ?
U3 O3B 1.854(13) . ?
U3 O9C 2.342(16) 10_566 ?
U3 O6C 2.389(14) . ?
U3 O8C 2.399(13) 10_566 ?
U3 O5C 2.462(17) 11_556 ?
U3 O4C 2.494(12) . ?
U3 U3 2.9184(19) 11_556 ?
U3 U4 3.0550(14) . ?
U4 O6C 1.605(18) . ?
U4 O4A 1.807(14) . ?
U4 O4B 1.866(13) . ?
U4 O12C 2.283(19) 11_556 ?
U4 O4C 2.345(10) . ?
U4 O6C 2.355(19) 11_556 ?
U4 O5C 2.365(14) . ?
U4 O7C 2.374(15) . ?
U4 O3C 2.382(19) . ?
U4 U4 2.8271(19) 11_556 ?
U4 U5 3.9763(12) . ?
U6 O6A 1.761(17) . ?
U6 O6B 1.844(15) . ?
U6 O16C 2.325(17) . ?
U6 O15C 2.336(14) . ?
U6 O13C 2.339(13) . ?
U6 O14C 2.396(14) . ?
U6 O10C 2.404(14) . ?
U6 O11C 2.414(14) . ?
U6 O12C 2.94(2) . ?
U5 O5B 1.767(14) . ?
U5 O5A 1.793(14) . ?
U5 O7C 2.27(2) . ?
U5 O8C 2.312(13) . ?
U5 O9C 2.326(13) . ?
U5 O9C 2.326(13) 11_556 ?
U5 O12C 2.332(14) . ?
U5 O12C 2.332(14) 11_556 ?
U5 O10C 2.370(13) . ?
U5 O10C 2.370(13) 11_556 ?
U5 O11C 2.383(12) 11_556 ?
U5 O11C 2.383(12) . ?
O11C O12C 1.10(2) . ?
O11C O10C 1.49(2) . ?
O16C O3C 1.16(3) 11_556 ?
O16C O15C 1.64(3) . ?
O16C U1 2.520(18) 11_556 ?
O15C U1 2.506(19) 11_556 ?
O14C O13C 1.53(3) . ?
O14C U1 2.445(17) 12_656 ?
O13C U1 2.461(14) 12_656 ?
O12C U4 2.283(19) 11_556 ?
O2C O2C 1.04(2) 2_655 ?
O2C O2C 1.04(2) 4_565 ?
O2C O2C 1.46(3) 3_665 ?
O2C U2 1.589(16) 4_565 ?
O2C U2 2.33(3) 3_665 ?
O2C U2 2.941(15) 2_655 ?
O1C U2 2.347(19) 4_565 ?
O3C O16C 1.16(3) 11_556 ?
O3C O4C 1.62(2) . ?
O6C O6C 1.05(3) 11_556 ?
O6C O5C 1.09(2) . ?
O6C O5C 1.62(3) 11_556 ?
O6C U4 2.355(19) 11_556 ?
O5C O5C 1.35(4) 11_556 ?
O5C O6C 1.62(3) 11_556 ?
O5C U3 2.463(17) 11_556 ?
O10C O9C 1.01(2) . ?
O9C O8C 1.78(2) . ?
O9C U3 2.342(16) 12_656 ?
O8C O9C 1.78(2) 11_556 ?
O8C U3 2.399(13) 12_656 ?
O8C U3 2.399(13) 2_655 ?
O7C U4 2.374(15) 11_556 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O1B U1 O1A 177.6(6) . . ?
O1B U1 O3C 91.0(6) . . ?
O1A U1 O3C 90.2(5) . . ?
O1B U1 O1C 93.1(6) . . ?
O1A U1 O1C 87.5(6) . . ?
O3C U1 O1C 135.5(8) . . ?
O1B U1 O4C 90.8(4) . . ?
O1A U1 O4C 88.7(5) . . ?
O3C U1 O4C 41.3(6) . . ?
O1C U1 O4C 175.0(6) . . ?
O1B U1 O14C 95.0(6) . 10_566 ?
O1A U1 O14C 82.6(5) . 10_566 ?
O3C U1 O14C 115.6(7) . 10_566 ?
O1C U1 O14C 108.2(8) . 10_566 ?
O4C U1 O14C 74.5(6) . 10_566 ?
O1B U1 O13C 93.1(6) . 10_566 ?
O1A U1 O13C 84.8(6) . 10_566 ?
O3C U1 O13C 151.8(7) . 10_566 ?
O1C U1 O13C 72.1(8) . 10_566 ?
O4C U1 O13C 110.8(6) . 10_566 ?
O14C U1 O13C 36.3(7) 10_566 10_566 ?
O1B U1 O15C 96.0(6) . 11_556 ?
O1A U1 O15C 86.4(5) . 11_556 ?
O3C U1 O15C 65.5(7) . 11_556 ?
O1C U1 O15C 70.0(8) . 11_556 ?
O4C U1 O15C 106.5(6) . 11_556 ?
O14C U1 O15C 168.9(5) 10_566 11_556 ?
O13C U1 O15C 141.4(6) 10_566 11_556 ?
O1B U1 O16C 94.7(6) . 11_556 ?
O1A U1 O16C 87.3(5) . 11_556 ?
O3C U1 O16C 27.5(6) . 11_556 ?
O1C U1 O16C 108.0(7) . 11_556 ?
O4C U1 O16C 68.5(5) . 11_556 ?
O14C U1 O16C 141.9(6) 10_566 11_556 ?
O13C U1 O16C 172.1(6) 10_566 11_556 ?
O15C U1 O16C 38.1(7) 11_556 11_556 ?
O1B U1 U2 72.9(4) . 4_565 ?
O1A U1 U2 106.7(4) . 4_565 ?
O3C U1 U2 153.0(5) . 4_565 ?
O1C U1 U2 29.9(5) . 4_565 ?
O4C U1 U2 155.1(3) . 4_565 ?
O14C U1 U2 87.8(5) 10_566 4_565 ?
O13C U1 U2 53.2(6) 10_566 4_565 ?
O15C U1 U2 94.2(5) 11_556 4_565 ?
O16C U1 U2 130.2(4) 11_556 4_565 ?
O1B U1 U2 74.4(4) . . ?
O1A U1 U2 107.1(4) . . ?
O3C U1 U2 112.6(5) . . ?
O1C U1 U2 29.0(5) . . ?
O4C U1 U2 150.8(3) . . ?
O14C U1 U2 130.7(5) 10_566 . ?
O13C U1 U2 95.3(6) 10_566 . ?
O15C U1 U2 52.0(5) 11_556 . ?
O16C U1 U2 87.4(4) 11_556 . ?
U2 U1 U2 42.85(3) 4_565 . ?
O2C U2 O2A 77.4(9) 2_655 . ?
O2C U2 O2B 103.2(10) 2_655 . ?
O2A U2 O2B 177.8(11) . . ?
O2C U2 O2C 21.7(10) 2_655 3_665 ?
O2A U2 O2C 86.9(8) . 3_665 ?
O2B U2 O2C 94.4(8) . 3_665 ?
O2C U2 O1C 93.0(11) 2_655 . ?
O2A U2 O1C 86.9(10) . . ?
O2B U2 O1C 90.9(7) . . ?
O2C U2 O1C 113.3(6) 3_665 . ?
O2C U2 O1C 95.9(11) 2_655 2_655 ?
O2A U2 O1C 87.4(10) . 2_655 ?
O2B U2 O1C 94.7(8) . 2_655 ?
O2C U2 O1C 76.7(6) 3_665 2_655 ?
O1C U2 O1C 168.2(5) . 2_655 ?
O2C U2 O2C 19.0(11) 2_655 . ?
O2A U2 O2C 87.4(9) . . ?
O2B U2 O2C 92.5(9) . . ?
O2C U2 O2C 36.0(7) 3_665 . ?
O1C U2 O2C 77.4(7) . . ?
O1C U2 O2C 112.7(6) 2_655 . ?
O2C U2 O2C 14.9(4) 2_655 4_565 ?
O2A U2 O2C 92.2(8) . 4_565 ?
O2B U2 O2C 88.5(8) . 4_565 ?
O2C U2 O2C 18.3(5) 3_665 4_565 ?
O1C U2 O2C 96.1(7) . 4_565 ?
O1C U2 O2C 94.5(7) 2_655 4_565 ?
O2C U2 O2C 19.1(4) . 4_565 ?
O2C U2 U2 51.3(10) 2_655 4_565 ?
O2A U2 U2 102.6(9) . 4_565 ?
O2B U2 U2 76.3(7) . 4_565 ?
O2C U2 U2 66.3(4) 3_665 4_565 ?
O1C U2 U2 50.9(5) . 4_565 ?
O1C U2 U2 140.8(5) 2_655 4_565 ?
O2C U2 U2 32.4(4) . 4_565 ?
O2C U2 U2 48.0(5) 4_565 4_565 ?
O2C U2 U2 53.9(9) 2_655 2_655 ?
O2A U2 U2 102.9(8) . 2_655 ?
O2B U2 U2 79.0(7) . 2_655 ?
O2C U2 U2 32.2(4) 3_665 2_655 ?
O1C U2 U2 140.8(5) . 2_655 ?
O1C U2 U2 50.8(5) 2_655 2_655 ?
O2C U2 U2 65.5(5) . 2_655 ?
O2C U2 U2 46.4(5) 4_565 2_655 ?
U2 U2 U2 90.0 4_565 2_655 ?
O2C U2 U1 121.5(10) 2_655 2_655 ?
O2A U2 U1 105.8(9) . 2_655 ?
O2B U2 U1 75.8(7) . 2_655 ?
O2C U2 U1 100.3(4) 3_665 2_655 ?
O1C U2 U1 144.8(4) . 2_655 ?
O1C U2 U1 29.2(4) 2_655 2_655 ?
O2C U2 U1 134.6(5) . 2_655 ?
O2C U2 U1 115.6(5) 4_565 2_655 ?
U2 U2 U1 147.79(3) 4_565 2_655 ?
U2 U2 U1 69.16(4) 2_655 2_655 ?
O2C U2 U1 117.5(10) 2_655 . ?
O2A U2 U1 105.6(9) . . ?
O2B U2 U1 72.3(6) . . ?
O2C U2 U1 134.2(4) 3_665 . ?
O1C U2 U1 28.4(4) . . ?
O1C U2 U1 145.9(4) 2_655 . ?
O2C U2 U1 99.5(4) . . ?
O2C U2 U1 115.9(5) 4_565 . ?
U2 U2 U1 68.00(4) 4_565 . ?
U2 U2 U1 147.07(3) 2_655 . ?
U1 U2 U1 117.34(3) 2_655 . ?
O5C U3 O3A 80.2(10) . . ?
O5C U3 O3B 102.7(9) . . ?
O3A U3 O3B 176.7(8) . . ?
O5C U3 O9C 144.3(9) . 10_566 ?
O3A U3 O9C 86.1(8) . 10_566 ?
O3B U3 O9C 90.6(7) . 10_566 ?
O5C U3 O6C 17.5(8) . . ?
O3A U3 O6C 91.3(8) . . ?
O3B U3 O6C 91.9(7) . . ?
O9C U3 O6C 160.3(6) 10_566 . ?
O5C U3 O8C 101.4(7) . 10_566 ?
O3A U3 O8C 84.6(8) . 10_566 ?
O3B U3 O8C 93.1(7) . 10_566 ?
O9C U3 O8C 44.2(5) 10_566 10_566 ?
O6C U3 O8C 116.1(5) . 10_566 ?
O5C U3 O5C 27.6(9) . 11_556 ?
O3A U3 O5C 91.4(9) . 11_556 ?
O3B U3 O5C 90.5(7) . 11_556 ?
O9C U3 O5C 121.6(6) 10_566 11_556 ?
O6C U3 O5C 38.9(6) . 11_556 ?
O8C U3 O5C 77.5(4) 10_566 11_556 ?
O5C U3 O4C 87.5(7) . . ?
O3A U3 O4C 91.7(8) . . ?
O3B U3 O4C 90.1(6) . . ?
O9C U3 O4C 126.0(5) 10_566 . ?
O6C U3 O4C 73.6(5) . . ?
O8C U3 O4C 169.6(3) 10_566 . ?
O5C U3 O4C 112.4(5) 11_556 . ?
O5C U3 U3 57.4(7) . 11_556 ?
O3A U3 U3 103.2(7) . 11_556 ?
O3B U3 U3 77.2(5) . 11_556 ?
O9C U3 U3 94.6(4) 10_566 11_556 ?
O6C U3 U3 67.0(4) . 11_556 ?
O8C U3 U3 52.5(2) 10_566 11_556 ?
O5C U3 U3 29.9(5) 11_556 11_556 ?
O4C U3 U3 137.8(2) . 11_556 ?
O5C U3 U4 48.8(6) . . ?
O3A U3 U4 108.3(6) . . ?
O3B U3 U4 75.0(5) . . ?
O9C U3 U4 163.9(5) 10_566 . ?
O6C U3 U4 31.4(4) . . ?
O8C U3 U4 141.7(2) 10_566 . ?
O5C U3 U4 66.6(3) 11_556 . ?
O4C U3 U4 48.7(2) . . ?
U3 U3 U4 89.15(2) 11_556 . ?
O6C U4 O4A 76.9(10) . . ?
O6C U4 O4B 106.4(9) . . ?
O4A U4 O4B 176.2(9) . . ?
O6C U4 O12C 148.8(8) . 11_556 ?
O4A U4 O12C 90.3(10) . 11_556 ?
O4B U4 O12C 86.0(9) . 11_556 ?
O6C U4 O4C 93.7(7) . . ?
O4A U4 O4C 90.9(7) . . ?
O4B U4 O4C 90.7(5) . . ?
O12C U4 O4C 115.1(6) 11_556 . ?
O6C U4 O6C 21.8(7) . 11_556 ?
O4A U4 O6C 85.5(9) . 11_556 ?
O4B U4 O6C 96.9(8) . 11_556 ?
O12C U4 O6C 130.9(6) 11_556 11_556 ?
O4C U4 O6C 113.8(5) . 11_556 ?
O6C U4 O5C 23.2(7) . . ?
O4A U4 O5C 89.6(9) . . ?
O4B U4 O5C 94.1(8) . . ?
O12C U4 O5C 170.9(7) 11_556 . ?
O4C U4 O5C 74.0(6) . . ?
O6C U4 O5C 40.0(6) 11_556 . ?
O6C U4 O7C 98.7(7) . . ?
O4A U4 O7C 79.6(9) . . ?
O4B U4 O7C 97.9(7) . . ?
O12C U4 O7C 50.6(6) 11_556 . ?
O4C U4 O7C 162.3(4) . . ?
O6C U4 O7C 80.6(5) 11_556 . ?
O5C U4 O7C 120.5(6) . . ?
O6C U4 O3C 132.6(8) . . ?
O4A U4 O3C 91.3(8) . . ?
O4B U4 O3C 87.8(7) . . ?
O12C U4 O3C 75.1(6) 11_556 . ?
O4C U4 O3C 40.0(5) . . ?
O6C U4 O3C 153.7(6) 11_556 . ?
O5C U4 O3C 114.0(7) . . ?
O7C U4 O3C 124.5(5) . . ?
O6C U4 U4 56.4(7) . 11_556 ?
O4A U4 U4 99.9(7) . 11_556 ?
O4B U4 U4 80.7(5) . 11_556 ?
O12C U4 U4 99.3(4) 11_556 11_556 ?
O4C U4 U4 143.9(3) . 11_556 ?
O6C U4 U4 34.6(4) 11_556 11_556 ?
O5C U4 U4 71.8(5) . 11_556 ?
O7C U4 U4 53.5(3) . 11_556 ?
O3C U4 U4 167.6(4) . 11_556 ?
O6C U4 U3 50.8(5) . . ?
O4A U4 U3 106.2(7) . . ?
O4B U4 U3 77.5(6) . . ?
O12C U4 U3 159.0(6) 11_556 . ?
O4C U4 U3 53.0(3) . . ?
O6C U4 U3 64.9(4) 11_556 . ?
O5C U4 U3 27.6(6) . . ?
O7C U4 U3 144.1(3) . . ?
O3C U4 U3 91.2(4) . . ?
U4 U4 U3 90.85(2) 11_556 . ?
O6C U4 U5 123.9(6) . . ?
O4A U4 U5 101.7(6) . . ?
O4B U4 U5 75.0(5) . . ?
O12C U4 U5 30.9(4) 11_556 . ?
O4C U4 U5 142.1(3) . . ?
O6C U4 U5 102.8(4) 11_556 . ?
O5C U4 U5 140.7(5) . . ?
O7C U4 U5 30.3(5) . . ?
O3C U4 U5 103.4(4) . . ?
U4 U4 U5 69.177(14) 11_556 . ?
U3 U4 U5 148.16(3) . . ?
O6A U6 O6B 177.6(7) . . ?
O6A U6 O16C 89.4(8) . . ?
O6B U6 O16C 88.9(6) . . ?
O6A U6 O15C 88.8(8) . . ?
O6B U6 O15C 88.8(6) . . ?
O16C U6 O15C 41.2(7) . . ?
O6A U6 O13C 88.9(10) . . ?
O6B U6 O13C 90.5(7) . . ?
O16C U6 O13C 120.3(7) . . ?
O15C U6 O13C 79.1(8) . . ?
O6A U6 O14C 87.6(9) . . ?
O6B U6 O14C 93.3(5) . . ?
O16C U6 O14C 157.7(7) . . ?
O15C U6 O14C 116.6(7) . . ?
O13C U6 O14C 37.6(7) . . ?
O6A U6 O10C 91.9(8) . . ?
O6B U6 O10C 90.4(6) . . ?
O16C U6 O10C 116.3(6) . . ?
O15C U6 O10C 157.4(7) . . ?
O13C U6 O10C 123.4(6) . . ?
O14C U6 O10C 85.9(6) . . ?
O6A U6 O11C 89.6(9) . . ?
O6B U6 O11C 91.7(5) . . ?
O16C U6 O11C 80.2(6) . . ?
O15C U6 O11C 121.4(7) . . ?
O13C U6 O11C 159.4(7) . . ?
O14C U6 O11C 121.8(6) . . ?
O10C U6 O11C 36.1(6) . . ?
O6A U6 O12C 103.7(9) . . ?
O6B U6 O12C 77.1(6) . . ?
O16C U6 O12C 65.7(6) . . ?
O15C U6 O12C 105.7(6) . . ?
O13C U6 O12C 166.4(6) . . ?
O14C U6 O12C 136.4(6) . . ?
O10C U6 O12C 52.3(5) . . ?
O11C U6 O12C 20.8(6) . . ?
O5B U5 O5A 179.8(7) . . ?
O5B U5 O7C 98.1(7) . . ?
O5A U5 O7C 81.7(9) . . ?
O5B U5 O8C 91.5(6) . . ?
O5A U5 O8C 88.7(8) . . ?
O7C U5 O8C 170.5(7) . . ?
O5B U5 O9C 88.0(5) . . ?
O5A U5 O9C 92.2(6) . . ?
O7C U5 O9C 134.7(5) . . ?
O8C U5 O9C 45.2(5) . . ?
O5B U5 O9C 88.0(5) . 11_556 ?
O5A U5 O9C 92.2(6) . 11_556 ?
O7C U5 O9C 134.7(5) . 11_556 ?
O8C U5 O9C 45.3(5) . 11_556 ?
O9C U5 O9C 90.2(10) . 11_556 ?
O5B U5 O12C 86.0(6) . . ?
O5A U5 O12C 93.9(7) . . ?
O7C U5 O12C 51.3(6) . . ?
O8C U5 O12C 130.0(5) . . ?
O9C U5 O12C 84.8(7) . . ?
O9C U5 O12C 172.2(7) 11_556 . ?
O5B U5 O12C 86.0(6) . 11_556 ?
O5A U5 O12C 93.9(7) . 11_556 ?
O7C U5 O12C 51.3(6) . 11_556 ?
O8C U5 O12C 130.0(5) . 11_556 ?
O9C U5 O12C 172.2(7) . 11_556 ?
O9C U5 O12C 84.8(7) 11_556 11_556 ?
O12C U5 O12C 99.7(10) . 11_556 ?
O5B U5 O10C 94.7(5) . . ?
O5A U5 O10C 85.3(5) . . ?
O7C U5 O10C 110.0(5) . . ?
O8C U5 O10C 69.0(4) . . ?
O9C U5 O10C 24.8(6) . . ?
O9C U5 O10C 114.2(7) 11_556 . ?
O12C U5 O10C 61.5(6) . . ?
O12C U5 O10C 161.0(7) 11_556 . ?
O5B U5 O10C 94.7(5) . 11_556 ?
O5A U5 O10C 85.3(5) . 11_556 ?
O7C U5 O10C 110.0(5) . 11_556 ?
O8C U5 O10C 69.0(4) . 11_556 ?
O9C U5 O10C 114.2(7) . 11_556 ?
O9C U5 O10C 24.8(6) 11_556 11_556 ?
O12C U5 O10C 161.0(7) . 11_556 ?
O12C U5 O10C 61.5(6) 11_556 11_556 ?
O10C U5 O10C 137.0(8) . 11_556 ?
O5B U5 O11C 97.8(4) . 11_556 ?
O5A U5 O11C 82.1(4) . 11_556 ?
O7C U5 O11C 73.4(4) . 11_556 ?
O8C U5 O11C 105.4(4) . 11_556 ?
O9C U5 O11C 150.4(7) . 11_556 ?
O9C U5 O11C 61.3(6) 11_556 11_556 ?
O12C U5 O11C 124.4(7) . 11_556 ?
O12C U5 O11C 26.9(6) 11_556 11_556 ?
O10C U5 O11C 166.4(6) . 11_556 ?
O10C U5 O11C 36.6(6) 11_556 11_556 ?
O5B U5 O11C 97.8(4) . . ?
O5A U5 O11C 82.1(4) . . ?
O7C U5 O11C 73.4(4) . . ?
O8C U5 O11C 105.4(4) . . ?
O9C U5 O11C 61.3(6) . . ?
O9C U5 O11C 150.4(7) 11_556 . ?
O12C U5 O11C 26.9(6) . . ?
O12C U5 O11C 124.4(7) 11_556 . ?
O10C U5 O11C 36.6(6) . . ?
O10C U5 O11C 166.4(6) 11_556 . ?
O11C U5 O11C 144.9(7) 11_556 . ?
O12C O11C O10C 135.7(15) . . ?
O12C O11C U5 73.9(9) . . ?
O10C O11C U5 71.2(6) . . ?
O12C O11C U6 108.0(15) . . ?
O10C O11C U6 71.6(8) . . ?
U5 O11C U6 123.7(5) . . ?
O3C O16C O15C 134.3(18) 11_556 . ?
O3C O16C U6 137.3(16) 11_556 . ?
O15C O16C U6 69.8(8) . . ?
O3C O16C U1 63.9(12) 11_556 11_556 ?
O15C O16C U1 70.5(9) . 11_556 ?
U6 O16C U1 125.2(7) . 11_556 ?
O16C O15C U6 69.0(9) . . ?
O16C O15C U1 71.4(10) . 11_556 ?
U6 O15C U1 125.3(8) . 11_556 ?
O13C O14C U6 69.2(7) . . ?
O13C O14C U1 72.4(9) . 12_656 ?
U6 O14C U1 123.2(7) . 12_656 ?
O14C O13C U6 73.2(8) . . ?
O14C O13C U1 71.3(8) . 12_656 ?
U6 O13C U1 125.0(6) . 12_656 ?
O11C O12C U4 161.8(12) . 11_556 ?
O11C O12C U5 79.1(9) . . ?
U4 O12C U5 119.0(8) 11_556 . ?
O11C O12C U6 51.2(12) . . ?
U4 O12C U6 119.2(8) 11_556 . ?
U5 O12C U6 106.0(7) . . ?
O2C O2C O2C 90.001(6) 2_655 4_565 ?
O2C O2C O2C 45.001(3) 2_655 3_665 ?
O2C O2C O2C 45.001(5) 4_565 3_665 ?
O2C O2C U2 124(3) 2_655 4_565 ?
O2C O2C U2 131(3) 4_565 4_565 ?
O2C O2C U2 148.9(7) 3_665 4_565 ?
O2C O2C U2 116.6(19) 2_655 3_665 ?
O2C O2C U2 34.6(18) 4_565 3_665 ?
O2C O2C U2 75(2) 3_665 3_665 ?
U2 O2C U2 96.5(11) 4_565 3_665 ?
O2C O2C U2 30.0(16) 2_655 . ?
O2C O2C U2 111.5(18) 4_565 . ?
O2C O2C U2 69.3(18) 3_665 . ?
U2 O2C U2 93.7(11) 4_565 . ?
U2 O2C U2 124.9(7) 3_665 . ?
O2C O2C U2 49.4(16) 2_655 2_655 ?
O2C O2C U2 45.0(15) 4_565 2_655 ?
O2C O2C U2 16.2(4) 3_665 2_655 ?
U2 O2C U2 133.1(9) 4_565 2_655 ?
U2 O2C U2 67.3(5) 3_665 2_655 ?
U2 O2C U2 66.5(4) . 2_655 ?
U1 O1C U2 122.6(8) . . ?
U1 O1C U2 120.9(8) . 4_565 ?
U2 O1C U2 78.3(5) . 4_565 ?
O16C O3C O4C 158.4(19) 11_556 . ?
O16C O3C U1 88.7(14) 11_556 . ?
O4C O3C U1 71.4(7) . . ?
O16C O3C U4 131.9(16) 11_556 . ?
O4C O3C U4 68.7(7) . . ?
U1 O3C U4 124.9(7) . . ?
O6C O6C O5C 97.9(13) 11_556 . ?
O6C O6C U4 123.6(7) 11_556 . ?
O5C O6C U4 121.4(17) . . ?
O6C O6C O5C 42.0(8) 11_556 11_556 ?
O5C O6C O5C 55.9(17) . 11_556 ?
U4 O6C O5C 144.6(16) . 11_556 ?
O6C O6C U4 34.6(4) 11_556 11_556 ?
O5C O6C U4 121.3(15) . 11_556 ?
U4 O6C U4 89.0(8) . 11_556 ?
O5C O6C U4 70.3(9) 11_556 11_556 ?
O6C O6C U3 113.0(4) 11_556 . ?
O5C O6C U3 23.6(13) . . ?
U4 O6C U3 97.9(7) . . ?
O5C O6C U3 73.0(8) 11_556 . ?
U4 O6C U3 124.2(8) 11_556 . ?
O6C O5C O5C 82.1(13) . 11_556 ?
O6C O5C U3 139(2) . . ?
O5C O5C U3 122.6(7) 11_556 . ?
O6C O5C O6C 40.1(14) . 11_556 ?
O5C O5C O6C 42.0(8) 11_556 11_556 ?
U3 O5C O6C 149.2(15) . 11_556 ?
O6C O5C U4 35.4(11) . . ?
O5C O5C U4 108.2(5) 11_556 . ?
U3 O5C U4 103.6(11) . . ?
O6C O5C U4 69.7(8) 11_556 . ?
O6C O5C U3 106.4(15) . 11_556 ?
O5C O5C U3 29.9(5) 11_556 11_556 ?
U3 O5C U3 92.7(8) . 11_556 ?
O6C O5C U3 68.1(8) 11_556 11_556 ?
U4 O5C U3 120.6(7) . 11_556 ?
O3C O4C U1 67.3(8) . . ?
O3C O4C U4 71.2(8) . . ?
U1 O4C U4 123.7(5) . . ?
O3C O4C U3 143.4(8) . . ?
U1 O4C U3 117.5(5) . . ?
U4 O4C U3 78.2(3) . . ?
O9C O10C O11C 146.2(14) . . ?
O9C O10C U5 75.1(10) . . ?
O11C O10C U5 72.2(6) . . ?
O9C O10C U6 122.1(17) . . ?
O11C O10C U6 72.3(8) . . ?
U5 O10C U6 124.8(6) . . ?
O10C O9C O8C 141.6(15) . . ?
O10C O9C U5 80.0(9) . . ?
O8C O9C U5 67.0(6) . . ?
O10C O9C U3 148.6(16) . 12_656 ?
O8C O9C U3 69.6(8) . 12_656 ?
U5 O9C U3 123.8(7) . 12_656 ?
O9C O8C O9C 134.8(11) . 11_556 ?
O9C O8C U5 67.8(5) . . ?
O9C O8C U5 67.8(5) 11_556 . ?
O9C O8C U3 66.2(5) . 12_656 ?
O9C O8C U3 136.0(10) 11_556 12_656 ?
U5 O8C U3 121.8(5) . 12_656 ?
O9C O8C U3 136.0(10) . 2_655 ?
O9C O8C U3 66.2(5) 11_556 2_655 ?
U5 O8C U3 121.8(5) . 2_655 ?
U3 O8C U3 74.9(5) 12_656 2_655 ?
U5 O7C U4 117.8(9) . 11_556 ?
U5 O7C U4 117.8(9) . . ?
U4 O7C U4 73.1(6) 11_556 . ?
 
_refine_diff_density_max    4.049
_refine_diff_density_min   -3.036
_refine_diff_density_rms    0.292

_shelxl_version_number 2014-1

